- Nano Review
- Open Access
Near-surface processing on AlGaN/GaN heterostructures: a nanoscale electrical and structural characterization
© Greco et al; licensee Springer. 2011
- Received: 30 September 2010
- Accepted: 11 February 2011
- Published: 11 February 2011
The effects of near-surface processing on the properties of AlGaN/GaN heterostructures were studied, combining conventional electrical characterization on high-electron mobility transistors (HEMTs), with advanced characterization techniques with nanometer scale resolution, i.e., transmission electron microscopy, atomic force microscopy (AFM) and conductive atomic force microscopy (C-AFM). In particular, a CHF3-based plasma process in the gate region resulted in a shift of the threshold voltage in HEMT devices towards less negative values. Two-dimensional current maps acquired by C-AFM on the sample surface allowed us to monitor the local electrical modifications induced by the plasma fluorine incorporated in the material.
The results are compared with a recently introduced gate control processing: the local rapid thermal oxidation process of the AlGaN layer. By this process, a controlled thin oxide layer on surface of AlGaN can be reliably introduced while the resistance of the layer below increase locally.
- Plasma Treatment
- Threshold Voltage
- Gate Bias
- Conductive Atomic Force Microscopy
Gallium nitride (GaN)-based heterostructures are promising materials for the fabrication of high-frequency and high-power devices. In particular, the presence of spontaneous and piezoelectric polarization charges in AlGaN/GaN layers leads to the appearance of a two dimensional electron gas (2DEG) at the AlGaN/GaN interface, typically having sheet carrier densities n s approximately 1 × 1013 cm-2 and high mobility (1,000-1,500 cm2/V s) . These properties make the materials suitable for the fabrication of transistors based on the 2DEG operating at high frequencies (up to tens of gigahertz), i.e., high-electron mobility transistors (HEMTs).
To date, for many applications, conventional AlGaN/GaN HEMTs have been fabricated as "depletion mode" transistors, i.e., these have a negative threshold voltage (V th) . However, the next generation of devices will require a more efficient use of the electric power. Hence, enhanced mode (normally-off) AlGaN/GaN HEMTs have become more desirable because these offer simplified circuitry (eliminating the negative power supply), in combination with favourable operating conditions for device safety.
Achieving reliable normally-off operation in AlGaN/GaN HEMTs is a challenging goal of current GaN technology. Several solutions, mostly involving nanoscale local modifications of the AlGaN barrier layer (e.g., recessed gate process , fluorine-based plasma etch , surface oxidation , etc.) have been recently proposed. Clearly, the transport properties of the 2DEG at AlGaN/GaN interfaces are strongly affected by those processes. In this context, using advanced nanoscale-resolution characterization methods can be the optimal way to monitor these local changes and to fully assess the basic transport phenomena in AlGaN/GaN heterostructures, in order to ultimately achieve reliable devices.
The accurate control of the threshold voltage (V th) is a key issue for normally-off HEMTs fabrication. In fact, several physical parameters affect the value of the threshold voltage V th, like the Schottky metal/semiconductor barrier height (Φ B ), the thickness of the AlGaN barrier layer (d), the residual doping concentration in the AlGaN (N D ), the polarization charge at the AlGaN/GaN interface (σ) or the concentration of charges intentionally introduced in the AlGaN barrier (N F ).
The introduction of negative charges in the near-surface region of the AlGaN barrier can be a possible method to monitor the carrier sheet concentration of the 2DEG and, hence, the value of V th. Based on this idea, Cai et al. demonstrated the possibility to shift the threshold voltage of AlGaN/GaN HEMTs to positive values by introducing fluorine ions by means of a reactive ion etching plasma process in CF4.. However, this process introduces a large amount of defects in the AlGaN barrier layer, which can lead to a degradation of the 2DEG mobility. Hence, an annealing process, after the gate fabrication, is needed to repair the damage and recover the mobility. The use of other plasma techniques, like inductive coupled plasma (ICP), could be also considered to reduce the damage and better control the parameters defining the normally-off operation (threshold voltage and sheet carrier concentration of the 2DEG).
A reduction of the barrier thickness d leads also to a positive shift of V th, as reported in the conventional approach of the recessed gate . Typically, recessed gate structures are formed by selective plasma etchings . However, etching just a few nanometers can be extremely difficult particularly considering a high reproducibility and wafer uniformity. Alternatively, Chang et al.  reported, in the case of AlN/GaN heterostructures, that a near surface oxidation process can be useful to convert into Aluminum oxide a surface-layer of AlN and, then, to reduce the thickness of the barrier layer below the critical thickness.
Other experiments investigated the effects of a thin oxide layer on the surface of AlGaN using a plasma treatment in O2 or in N2O . In this context, the effects of a rapid thermal oxidation on the surface were not addressed yet.
In this context, this work studies the effects of near-surface processing on the properties of AlGaN/GaN heterostructures, combining conventional electrical analyses of HEMTs with advanced nanoscale characterization techniques as transmission electron microscopy (TEM), atomic force microscopy (AFM) and conductive atomic force microscopy (C-AFM). In particular, nanoscale current measurements demonstrated a local reduction of the leakage currents (i.e., an increasing of the resistance of the material) both using a CHF3 plasma or rapid oxidation treatments of the surface. Hence, these processes could find interesting applications in the fabrication of innovative GaN-based transistors.
AlGaN/GaN heterostructures grown on different substrates (SiC, Si, Al2O3) were used in our experiments. In order to determine the physical properties of the 2DEG, HEMTs devices with an appropriate geometry were fabricated. First, reference HEMT devices (i.e., not subjected to the plasma treatment) were fabricated. Source and drain Ohmic contacts were formed by an annealed Ti/Al/Ni/Au multilayer  and the gate Schottky contact was subsequently formed by a Pt/Au bilayer . To study the effect of the plasma treatment on the 2DEG transport properties, the region where the gate electrode had to be fabricated was modified (before metal deposition) with a plasma process using a CHF3/Ar gas mixture, as schematically illustrated in Figure 1b. The plasma treatment was performed at room temperature using the Roth & Rau Microsys 400 ICP equipment. The CHF3/Ar gas flux was 20 sscm and the operating pressure in the chamber was 5 × 10-2 mbar. The control bias, the power, and the process duration were 200 V, 250 W and 300 s, respectively. Afterwards, the Pt/Au gate electrode was formed on the same region subjected to plasma treatment, using a self-aligned process and lift-off technique for metal definition. Finally, the sample was subjected to an annealing process at 400°C, in order to recover the damage induced by the plasma process. It is worth noting that this annealing process does not cause degradation of the gate Schottky contact.
In order to characterize the physical properties of the 2DEG, both macroscopic and nanoscale electro-structural analysis of the near-surface region of the samples were performed. First, current-voltage (I-V) and capacitance-voltage (C-V) measurements of HEMT devices were performed in a Karl Süss probe station, equipped with a parameter analyzer. These macroscopic electrical measurements gave information on the current flowing in the 2DEG, allowing also to determine the threshold voltage and the sheet carrier density in the 2DEG. Then, TEM analysis was used to monitor the heterojunction microstructure and the crystalline defects. AFM and C-AFM were used to study the sample morphology as well as the local electrical behaviour of the modified surface region.
Finally, a preliminary investigation on the effect of a near-surface oxidation process was performed. For this aim, a rapid thermal oxidation (RTO) at 900°C for 10 min was carried out in a Jipelec JetFirst furnace. The nanoscale electro-structural properties of the oxidized region were characterized by means of TEM, AFM and C-AFM.
Figure 1c shows the I DS-V GS characteristics for different gate biases V GS, in the case of a reference untreated (as prepared) HEMT device (squares) and for a device subjected to a CHF3 plasma treatment (circles). For the untreated device a saturation current of 2.2 mA is reached at a gate bias V GS = 0, while at the same gate voltage (V GS = 0) the saturation current decreases to 0.15 mA in the CHF3-treated device. It is worth noting that a positive gate bias of +2 V must be applied to the HEMT subjected to CHF3 treatment to achieve a saturation current value of 2.4 mA, comparable with that in the untreated device at V GS = 0 V. Furthermore, the gate bias necessary to reduce I DS to a value of 10 nA changes from -2 to -0.5 V, from the untreated to the plasma-treated device. Finally, for a fixed gate bias of -2 V the leakage current decreases from 10 to 0.5 nA, after the plasma treatment.
Moreover, from the values of source-gate current I GS (not showed) we observed a decrease of the current of leakage for the plasma-treated device under reverse bias. In particular, at V GS = -10 V the leakage current was reduced from 100 to 10 nA. The decrease in the reverse leakage current was also accompanied by a reduced forward current (i.e., from 10 to 4 mA at V GS = +3 V), most probably due to an increase of the series resistance. The decreasing of the leakage current can be due to several reasons: (1) an increase of the Schottky barrier height, (2) the depletion of the 2DEG channel, and (3) an increase in the resistivity in the upper shallow AlGaN layer due to lattice damage.
Figure 4b reports the AFM morphological image of the sample. As can be seen, no substantial difference can be observed between stripes processed with CH3 plasma and stripes without any treatment. On the other hand, a significant difference can seen by the transversal current map acquired by C-AFM and shown in Figure 4c. This picture clearly shows the electrical changes of the material due to the plasma treatment. The local current is significantly reduced (two orders of magnitude) on the stripes processed with plasma, with respect to the ones without plasma treatment. This behaviour is consistent with an increased local resistance in the plasma-etched regions, which in turn can be associated whether to a partial depletion of the 2DEG channel or more simply to an increase of the local resistance of the AlGaN barrier layer due to plasma-induced damage.
The experimental results found from the macroscopic I-V characteristic of the devices and the nanoscale electro-structural analysis of the near-surface region suggest that the observed electrical modifications are due both to the introduction of negative fluorine ions (as already reported in the literature) but also to the plasma-induced damage.
The near-surface modification induced by a RTO process was also monitored by combining TEM and scanning probe microscopy techniques.
Similarly to the case of the sample treated with plasma, also in the oxidized sample we prepared a sample for local electrical characterization. The sample consisted of regions (stripes) of locally oxidized material alternating with non-oxidized material. As can be seen, while the morphology of the oxidized regions remains practically unchanged with respect to the non-oxidized ones (Figure 6a), the current flow through the 2DEG was locally suppressed in the oxidized regions, which in turn exhibit a more resistive behaviour (Figure 6b).
Hence, this selective local oxidation process can be potentially useful to tailor the electrical properties of AlGaN barrier layers and/or as a novel approach for recessed-gate or insulated-gate technology for normally-off GaN HEMTs.
In summary, a nanoscale approach was used to monitor the impact of near-surface processing on the electrical and structural properties of AlGaN/GaN heterostructures. The introduction of defects and/or negative charges by the CHF3 into the GaN (or AlGaN/GaN heterostructure) was deduced by TEM and C-AFM and can be indicated as the main cause of the depletion of the 2DEG and shift of the threshold voltage in HEMT devices.
A local increase of the resistivity was observed by a rapid thermal oxidation of the sample, which led to the formation of a very thin surface oxide. In this perspective, the nanoscale comprehension of the effects associated to the CHF3 plasma treatment and to oxidation processes can be useful to design and fabricate normally-off devices, with an insulated gate technology.
The authors thank S. Di Franco for clean room samples processing and C. Bongiorno for technical assistance and discussions during TEM analysis.
This work was supported by ST Microelectronics-Catania and by the FIRB project RBIP068LNE_001 of the Italian Ministry for Research.
- Ambacher O, Smart J, Shealy JR, Weimann NG, Chu K, Murphy M, Schaff WJ, Eastman LF: Two-dimensional electron gases induced by spontaneous and piezoelectric polarization charges in N- and Ga-face AlGaN/GaN heterostructures. J Appl Phys 1999, 85: 3222. 10.1063/1.369664View ArticleGoogle Scholar
- Brennan KF, Brown AS: Theory of modern electronic semiconductor devices. New York: Wiley; 2002.View ArticleGoogle Scholar
- Landford WB, Tanaka T, Otoki Y, Adesida I: Recessed-gate enhancement-mode GaN HEMT with high threshold voltage. Electronics Lett 2005., 41: Google Scholar
- Cai Y, Zhou Y, Lau KM, Chen KJ: Control of Threshold Voltage of AlGaN/GaN HEMTs by Fluoride-Based Plasma Treatment: From Depletion Mode to Enhancement Mode. IEEE Trans Electron Devices 2006, 53(9):2207. 10.1109/TED.2006.881054View ArticleGoogle Scholar
- Tajima M, Kotani J, Hashizume T: Effects of Surface Oxidation of AlGaN on DC Characteristics of AlGaN/GaN High-Electron-Mobility Transistors. Jpn J Appl Phys 2009, 48: 020203. 10.1143/JJAP.48.020203View ArticleGoogle Scholar
- Lorenz A, Derluyn J, Das J, Cheng K, Degroote S, Medjdoub F, Germain M, Borghs G: Influence of thermal anneal steps on the current collapse of fluorine treated enhancement mode SiN/AlGaN/GaN HEMTs. Phys Status Solidi 2009, C6: S996-S998.View ArticleGoogle Scholar
- Saito W, Takada Y, Karaguchi M, Tsuda K, Omura I: Recessed-Gate Structure Approach Toward Normally Off High-Voltage AlGaN/GaN HEMT for Power Electronics Applications. IEEE Trans Electron Devices 2006, 53: 356. 10.1109/TED.2005.862708View ArticleGoogle Scholar
- Chang CY, Pearton SJ, Lo CF, Ren F, Kravchenko II, Dabiran AM, Wowchak AM, Cui B, Chow PP: Development of enhancement mode AlN/GaN high electron mobility transistors. Appl Phys Lett 2009, 94: 263505. 10.1063/1.3168648View ArticleGoogle Scholar
- Roccaforte F, Giannazzo F, Iucolano F, Raineri V: Nanoscale carrier transport in Ti/Al/Ni/Au Ohmic contacts on AlGaN epilayers grown on Si(111). Appl Phys Lett 2006, 89: 022103. 10.1063/1.2220486View ArticleGoogle Scholar
- Chu R, Chu R, Suh CS, Wong MH, Fichtenbaum N, Brown D, McCarthy L, Keller S, Wu F, Speck JS, Mishra UK: Impact of CF4 Plasma Treatment on GaN. IEEE Electron Device Lett 2007, 28: 781. 10.1109/LED.2006.889238View ArticleGoogle Scholar
- Roccaforte F, Giannazzo F, Iucolano F, Raineri V: Electrical behavior of AlGaN/GaN heterostuctures upon high-temperature selective oxidation. J Appl Phys 2009, 106: 023703. 10.1063/1.3174438View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.